### University of Strathclyde

### Department of Mechanical Engineering

## Novel computational methods to predict the deformation of macroscopic

## heterogeneous materials

### A. J. Beveridge

### A thesis presented in fulfilment of the requirements for the degree of Doctor of Philosophy

### 2011

This thesis is the result of the author’s original research. It has been composed by the author and has not been previously submitted for examination which has led to the award of a degree.

The copyright of this thesis belongs to the author under the terms of the United Kingdom Copyright Acts as qualified by University of Strathclyde Regulation 3.50. Due acknowledgement must always be made of the use of any material contained in, or derived from, this thesis.

Signed: Date:

## Acknowledgements

I must give special thanks to Dr Wheel for his diligent supervision. It was always an encouragement to know someone else was thinking about my work, willing to throw ideas around and steer the work in the right direction. Thanks also to Dr Nash for his pastoral support, particularly in the last year when employment took me away from Glasgow. And finally to Andy Crockett for helping with the experimental testing, Tommy Sherwood for the design and preparation of the aluminium model material and Afan Waseem for the experimental acrylic ring results.

To name and thank all who have given me support and help throughout the PhD, to repay their time in equal measure with the words about them, would take many times the length of this thesis.

Whether I have written many words about you, just a few or none at all, please know that I am very grateful to everyone who listened and humoured me through- out the ups and downs of these past years.

Thank you.

These words have been my goal:

“What ever you do work heartily, as for the Lord and not for men, knowing that from the Lord you will receive the inheritance as your reward. You are serving

the Lord Christ”

Colossians 3:23-24 (ESV)

## Contents

1 Introduction 2

1.1 Experimental Methods in Micropolar

Elasticity . . . 4

1.2 Numerical Methods in Micropolar Elasticity . . . 7

1.3 Research Aims . . . 9

2 Micropolar Elasticity 12 2.1 Generalised Linear Micropolar Elasticity . . . 12

2.2 Two Dimensional Formulations . . . 14

2.2.1 Plane Strain . . . 17

2.2.2 Plane Stress . . . 18

2.3 One Dimensional Formulations . . . 19

2.3.1 Slender Beam . . . 19

2.3.2 Thin Walled Ring . . . 23

2.4 Conclusion . . . 25

3 Model Material - Slender Beam 27

3.1 Experimental Procedure . . . 30

3.2 Detailed Finite Element Analysis . . . 33

3.3 Results . . . 39

3.4 One Dimensional Beam Finite Element . . . 42

3.4.1 Validation . . . 44

3.4.2 Slender Beam Comparison . . . 45

3.5 Conclusion . . . 47

4 Control Volume Finite Element Method 49 4.1 Discrete Kirchhoff Triangular Element . . . 50

4.2 Micropolar Linear Strain Triangular Element . . . 51

4.2.1 Control Volume Formulation . . . 55

4.2.2 Validation . . . 61

4.3 Conclusion . . . 70

5 Model Material - Deep Beam 71 5.1 Experimental Results . . . 73

5.2 Iterative Constitutive Code . . . 79

5.2.1 Procedure . . . 79

6 Model Material - Diametrically Loaded Ring 86 6.1 Constitutive Properties . . . 89

6.2 Discussion . . . 90

7 Summary and Conclusions 93 A Discrete Kirchhoff Triangular Element 97 A.1 Mindlin Plate Bending Theory . . . 97

A.1.1 Deformations . . . 97

A.1.2 Moment Curvature Relations . . . 98

A.1.3 Equilibrium . . . 99

A.2 DKT Element . . . 99

A.3 Element Stiffness Matrix . . . 102

A.3.1 Finite Element Method . . . 102

A.3.2 Control Volume Finite Element Method . . . 103

A.4 Boundary Conditions and Solution . . . 107

A.5 Results . . . 107

A.5.1 Patch Test . . . 108

A.5.2 Uniformly Distributed Load (UDL) . . . 109

A.5.3 Centrally Applied Load . . . 109

A.5.4 Boundary Conditions . . . 111

A.6 Conclusion . . . 111

B MATLAB Control Volume Finite Element Codes 117 B.1 CV-DKT . . . 117

B.2 CV-MPLST . . . 123

C MATLAB Iterative Constitutive Code 132 C.1 MicropolarBeamREGbeta Code . . . 132

D Ansys Discrete Detail Input Files 136

D.1 HMD Geometry Input B1 . . . 136 D.2 LMD Geometry Input B1 . . . 138

## List of Figures

2.1 Micropolar differential stress element . . . 15

2.2 Deformation of stress element due to antisymmetric, τa, and sym- metric, τs, shear stresses . . . 16

2.3 Stress acting upon a one dimensional micropolar beam . . . 20

2.4 Model beam subjected to three point bending . . . 21

2.5 Model ring subject to diametrically opposing point loads . . . 23

3.1 Diagram of hole pitch with horizontal pitch P_{1} and vertical pitch P_{2} 28
3.2 Photograph of HMD test pieces . . . 29

3.3 (a) LMD B1 in three point bending with cross head measurement only (b) HMD B1 in three point bending with independent central defection reading from extensometer . . . 31

3.4 Test data plot from Microsoft Excel showing load displacement curve for HMD B1 10 with fitted straigh line and equation of straight line shown with gradient highlighted in box . . . 32

3.5 Diagram showing relative crosshead and rig flexure displacements
for three point bending experimental procedure . . . 32
3.6 Stiffness against 1/depth^{2} for HMD beams at L/d = 10.08. Com-

paring discrete detail ANSYS, experimental results and experimen- tal results corrected for test rig flexure against classical solution . 33

3.7 Stiffness against 1/depth^{2} for LMD beams at L/d = 9.92. Compar-
ing discrete detail ANSYS, experimental results and experimental
results corrected for test rig flexure against classical solution . . . 34
3.8 Flow chart showing the sequence of steps used to create the de-

tailed finite element beam geometry . . . 35 3.9 Array of unit cells and half unit cells to create detailed beam ge-

ometry . . . 36 3.10 Convergence of absolute central deflection against number of nodes

for HMD B1 10 geometery, comparing ANSYS elements 182 and 183 . . . 37 3.11 Convergence of absolute central deflection against number of nodes

for LMD B1 10 geometery, comparing ANSYS elements 182 and 183 37 3.12 Quarter mesh for HMD discrete detail finite element model. Mesh

refinement parameter refine= 1, 378 nodes . . . 38 3.13 Quarter mesh used in LMD discrete detail finite element model.

Mesh refinement parameter refine= 0.5, 62 nodes . . . 39 3.14 Beam element . . . 43 3.15 Tip displacement convergence to couple stress beam theory for

cantilever beam at various depth to characteristic length ratios . . 45 3.16 Stiffness result from Micropolar Beam element (EXPBeamE) for a

given load (100N ). Plotted against stiffness from the experimental procedure (EXP). . . 46 3.17 Stiffness result from Micropolar Beam element (ANSYSBeamE)

for a given load (100N ). Plotted against displacements gained from the ANSYS procedure (ANSYS). . . 46

4.1 Six node quadratic displacement triangular element . . . 52

4.2 Dual control volume mesh constructed around the vertices of a six node triangular finite element mesh . . . 55 4.3 Sign convension for dual mesh on a single finite element mesh . . 56 4.4 Element stress resultants working on the face of the control volume 58 4.5 Mesh for micropolar element patch test, lengths in (mm) . . . 62 4.6 Stress concentration mesh 8x15x4 r = 0.864mm. Quarter plate

edge lengths are 16.2mm x 16.2mm. . . 65 4.7 Convergence to slender beam solution for increasing degrees of free-

dom . . . 68 4.8 Time to solution for slender beam solution for increasing degrees

of freedom . . . 68 4.9 Unit beam mesh . . . 69

5.1 Stiffness against 1/depth^{2} at L/d = 7.56 for various coupling num-
bers with material properties from slender HMD beams . . . 72
5.2 Stiffness against 1/depth^{2} at L/d = 5.04 for various coupling num-

bers with material properties from slender HMD beams . . . 72
5.3 Stiffness against 1/depth^{2} for HMD beams at L/d = 7.56. Com-

paring discrete detail ANSYS and experimental results corrected
for test rig flexure against classical solution . . . 76
5.4 Stiffness against 1/depth^{2} for HMD beams at L/d = 5.04. Com-

paring discrete detail ANSYS and experimental results corrected
for test rig flexure against classical solution . . . 76
5.5 Stiffness against 1/depth^{2} for LMD beams at L/d = 8.50. Com-

paring discrete detail ANSYS and experimental results corrected for test rig flexure against classical solution . . . 77

5.6 Stiffness against 1/depth^{2} for LMD beams at L/d = 5.67. Com-
paring discrete detail ANSYS and experimental results corrected
for test rig flexure against classical solution . . . 77
5.7 Unit mesh used for HMD L/d=10.08 . . . 80
5.8 Best fit solutions for HMD samples based upon the ANSYS results

at the three different spans after the first iteration to find the
coupling number N using L/d = 5.04, R^{2} = 0.93 at this span . . . 82
5.9 Flow chart showing iterative process to find the best fit material

parameters for the HMD model material . . . 83 5.10 Best fit solutions for HMD samples based upon the ANSYS results

at the three different spans after the second iteration to find the
couple modulus γ using L/d = 10.08, R^{2} = 0.99 at this span . . . 84
5.11 Variation of stiffness for ± 15% Poisson’s ratio for different spans

HMD . . . 85

6.1 Model ring of radius R and depth d with radial void distribution dimensions of pitch n, pitch radius rn, initial offset angle θni and offset angle θn . . . 87 6.2 Best fit solution for ring samples based upon experimental stiffness

results . . . 90 6.3 Flow chart showing iterative process to find the best fit material

parameters from the model ring experimental results . . . 92

A.1 Differential plate element undeformed (a) and deformed plate(b) . 98 A.2 Transition to the DKT element. (a) 6 noded Mindlin element with

the triangular area coordinates δ, ξ and η. (b) 3 noded DKT element with vertex node degrees of freedom (wi, w,xi w,yi) . . 100

A.3 (a) Control volume dual mesh centred on finite element node P (b) Equilibrium of forces acting upon a differential line dr along the control volume face . . . 103 A.4 (a) Element coordinate systems: global Cartesian, line and area.

Element and control volume node labelling convention (b) Specific area coordinates relating to element and control volume nodes . . 106 A.5 Triangular mesh of 2x2 square plate of dimensions a and b . . . . 108 A.6 Patch test mesh . . . 109 A.7 Central deflection convergence to thin plate theory. Hard clamped

with uniform load, a/b = 1 and h = 0.05 . . . 112 A.8 Central deflection convergence to thin plate theory. Soft clamped

with uniform load, a/b = 1 and h = 0.05 . . . 112 A.9 Central deflection convergence to thin plate theory. Hard simply

supported with uniform load, a/b = 1 and h = 0.05 . . . 113 A.10 Central deflection convergence to thin plate theory. Soft simply

supported with uniform load, a/b = 1 and h = 0.05 . . . 113 A.11 Central deflection convergence to thin plate theory. Hard clamped

with central point load, a/b = 1 and h = 0.05 . . . 114 A.12 Central deflection convergence to thin plate theory. Soft clamped

with central point load, a/b = 1 and h = 0.05 . . . 114 A.13 Central deflection convergence to thin plate theory. Hard simply

supported with central point load, a/b = 1 and h = 0.05 . . . 115 A.14 Central deflection convergence to thin plate theory. Soft simply

supported with central point load, a/b = 1 and h = 0.05 . . . 115 A.15 Convergence of rotation about the normal along plate boundary for

CVFEM. Soft simply supported with central point load, a/b = 1 and h = 0.05 . . . 116

A.16 Convergence of rotation about the normal along plate boundary for FEM. Soft simply supported with central point load, a/b = 1 and h = 0.05 . . . 116

## List of Tables

3.1 Hole radius, r, horizontal, P1, and vertical pitch, P2, for model material, see figure 3.1 . . . 30 3.2 Beam dimensions for HMD and LMD test pieces . . . 30 3.3 Beam test geometry and corrected stiffness results,K, for HMD

and LMD test pieces . . . 40 3.4 Constitutive properties for HMD slender beams. Flexural modulus

E_{f m}, couple modulus γ and characterisitc length of bending l_{b} . . 41
3.5 Constitutive properties for LMD slender beams. Flexural modulus

Ef m, couple modulus γ and characterisitc length of bending lb . . 41 3.6 Tip displacement for finite element micropolar beam compared

against exact analytical solution for an end moment and a point load . . . 44

4.1 Vertex coordinates, in triangular area coordinates, for the inter- connecting control volume (CV) of a six node triangular element shown in figure 4.3 . . . 56 4.2 Substitutions for the equilibrium equation integrals and stress dis-

placement relationships . . . 60 4.3 Body and boundary loadings and displacement field solutions for

micropolar element patch test. . . 63

4.4 Vertex coordinates and constitutive properties for micropolar ele- ment patch test . . . 63 4.5 Results for displacement and micro rotation at node 2. Stress and

couple stress at point P in the patch test mesh under loading cases 1 and 2 . . . 64 4.6 Results for displacement and micro rotation at node 2. Stress and

couple stress at point P in the patch test mesh under loading case 3. Results shown against exact solution for linear strain control volume CV-MPLST and constant strain control volume CV-MPCST 64 4.7 Stress concentration factors for maximum circumferential stress at

circular hole by the constant strain control volume, CV-MPCST, linear strain control volume, CV-MPLST, constant strain finite element, FE-MPCST, and linear strain finite element, FE-MPLST.

Hole radius 0.216mm, Gm =1.0e9N/m^{2}, νm = 0.3 and (A):^{r}_{l} =
1.063 (B):^{r}_{l} = 10.63. Mesh is 8x22x4 elements. . . 66
4.8 Stress concentration factors for maximum circumferential stress at

circular hole by the constant strain control volume, CV-MPCST, linear strain control volume, CV-MPLST, constant strain finite element, FE-MPCST, and linear strain finite element, FE-MPLST.

Hole radius 0.864mm, Gm =1.0e9N/m^{2}, νm = 0.3 and a = 0.3333.

Mesh is 8x15x4 elements. . . 67

5.1 Beam test geometry and corrected stiffness results, K, for deep HMD test pieces . . . 74 5.2 Beam test geometry and corrected stiffness results, K, for deep

LMD test pieces . . . 75

6.1 Geometric data for ring samples . . . 88 6.2 Experimental stiffness results,K, for ring samples at two aspect

ratios; R/d = 8 and R/d = 4 . . . 89

A.1 Substitutions for the discrete equation integrals and moment cur- vature matrix . . . 105 A.2 Patch test results for a state of pure bending and twist, where wn

is the transverse displacement of node n and Mx, My and Mxy are the x bending moments, y bending moments and twisting moments respectively. Moments were calculated at the element centroids. . 110

## List of Symbols

### Math Symbols

[] matrix, row vector {} column vector δij Kronecker delta eijk permutation tensor

### Latin Symbols

a coupling factor

A area

b beam breadth

B spatial derivates of field variables

d beam depth

d nodal displacement vector D constitutive property

D constitutive property matrix E Young’s modulus

Em micropolar Young’s modulus Ef m micropolar flexural modulus F force resultant

Gm observed micropolar shear modulus H modified shape function vector

I second moment of area k element stiffness matrix K bending stiffness

K global stiffness matrix l control volume face length lb characteristic length of bending lt characteristic length of torsion L beam length

mij couple stress tensor M applied bending moment

M bending moment vector, couple resultant n normal coordinate

n number of nodes

N coupling number, shape function N shape function vector

p body force per unit volume P1 horizontal void pitch P2 vertical void pitch P applied load vector

q body couple per unit volume r void radius, line coordinate R radius of curvature

R^{2} coefficient of multiple determination
s tangent coordinate

SSerr sum of the squared residual errors SStot sum of the squared total errors T shear force per unit length T shear force vector

u displacment in x direction uij displacement vector v displacment in y direction w displacment in z direction W applied load

x Cartesian coordinate

y Cartesian coordinate

z Cartesian coordinate, plate thickness

### Greek Symbols

α micropolar elastic constant β micropolar elastic constant

γ micropolar couple modulus, shear strains δ triangular area coordinate

ǫ direct strains

η triangular area coordinate εij strain tensor

θ macro rotation

κ micropolar elastic constant
λ micropolar Lame’s constant
µ observed shear modulus
µ^{∗} micropolar shear modulus
ν Poisson’s ratio

νm micropolar Poisson’s ratio ξ triangular area coordinate τij force stress tensor

φ micro rotation χ curvature vector Ψ polar ratio

## Abstract

Heterogeneous materials can exhibit behaviour under load that cannot be de- scribed by classical continuum elasticity. Beams in bending can show a relative stiffening as the beam depth tends to zero, a size effect. Size effects are recog- nised in higher order continuum elastic theories such as micropolar elasticity. The drawback of higher order theories is the requirement of addition constitutive rela- tions and associated properties that are often difficult to establish experimentally.

Furthermore the finite element method, of great benefit in classical elasticity, has shown limitations when applied to micropolar elasticity. The determination of additional constitutive properties and the numerical modelling of micropolar elas- ticity is discussed in the context of two model heterogeneous materials.

The first model material was created by drilling holes in an aluminium bar in a regular pattern, with the hole axis normal to the plane of bending. Bending tests show that a size effect is present. These results are compared against a model of the detailed beam geometries in the finite element package ANSYS, which confirms the size effect. Constitutive properties are extracted from the ANSYS results in a new iterative procedure using approximate numerical solutions from a newly developed control volume finite element. This iterative procedure is then used to obtain constitutive properties from the second model material tested as diametrically loaded acrylic rings, with a material size scale equal to a quarter of that of the perforated aluminium beams.

Despite difficulties, associated with the anisotropic nature of the model materials, micropolar elasticity will be shown to be capable of modelling the size effects identified in these model materials.

## Chapter 1 Introduction

Considering Scale

It is clear from observing any material that, from a sufficiently far distance, it can appear as of one phase, a homogeneous continuum. On magnifying the ma- terial, however, it can be seen that it is in fact made up of a number of phases.

This scale effect is dependent upon the material. For example, steel would re- quire to be magnified to a micro metre level to notice the different constituent phases of its microstructure, whereas the microstructure of polymeric foam can be seen with the naked eye. All materials are heterogeneous but it depends upon the scale at which they are observed whether this is significant. As scale has an effect upon what is observed so has it upon the deformation of the material under load. At a macroscopic level steel is classed as being homogenous and thus the deformation can be described by classical continuum elasticity. On a micro- scopic level, however, the deformation becomes dependent upon the individual responses of the phases and their interactions. In many respects the macroscopic response, characterised by a classical continuum, is an averaging of the micro- scopic response, but when the overall deformation is occurring on a scale similar to that of the microstructure then a different approach to classical elasticity may be required. This has become an engineering challenge due to the increased use of heterogeneous materials in structural applications [1]. For example, polymeric and metallic foams, particularly as part of sandwich panels, are now being used

more extensively in both automotive and aerospace applications because of the weight saving they afford [1]. It is an active research area to find constitutive models that can describe the elastic response of these materials as they are often endowed with enhanced mechanical behaviour, which are termed size effects [2]

due the dependence of this behaviour upon the size of the material domain.

Generalised Elastic Continua

Classical elasticity [3] is a local theory; the forces acting upon an individual point depend only upon its location. Non local theories take note of effects neighbouring that point and how these affect the forces acting upon it. Therefore the deformation of an individual element is now dependant upon its location and neighbourhood. Intrinsic length scales link the two effects. As the problem domain approaches the length scale the non local effect will increase. Conversely as the domain expands away from the length scale the local effects dominate and a local continuum approach is sufficient.

In elasticity non-local effects can be expressed within a continuum by gener- alised elasticity, or non-local elasticity, of which there are two different classes;

higher grade and higher order [2]. Higher grade theories incorporate higher or additional derivatives of the displacement vector whereas higher order theories include additional microstructural degrees of freedom. Couple stress theory [4] is an example of a higher grade theory. An example of a higher order theory is the linear micropolar theory [5]. Linear micropolar theory is endowed with only one additional degree of freedom, a micro rotation, and is therefore the least complex of the higher order theories.

As with many of the generalised elastic theories these two different approaches are linked. If the additional micro rotation of micropolar elasticity is no longer kinematically distinct, equalling the macro rotation, then we have couple stress theory. There are numerous other generalised theories with greater complexity than couple stress or micropolar elasticity. The historical development of gener- alised theories has been discussed at length in the literature and the reader can be directed to [2, 6–8], and references therein for an overview.

This work is concerned with the simplest of the higher order theories, micropolar elasticity. An additional independent micro rotation is present in the formulation, enabling the complimentary shear stress requirement of classical elasticity to be relaxed. Additional couple stresses balance the differential element. The couple stresses have an intrinsic length scale associated with them. Endowed with this additional degree of freedom micropolar elasticity predicts elastic behaviour that is not predicted by classical elasticity. For example the dispersion of stress waves, a dependence of stress concentration factors upon discontinuity size and a size stiffening of smaller samples in bending and torsion are all predicted. The pre- diction of these additional material behaviours led to research into experimental identification of these size effects and the determination of the additional con- stitutive properties associated with the theory. To date this has proved to be a challenging task.

### 1.1 Experimental Methods in Micropolar Elasticity

“...experiments with micropolar constants require much precision and elaborate instrumentation, since we are faced with the measurements of microscopic-level quantities ... At this range, many other physical phenomenon begin to interfere

with observation, introducing distortions and errors.” Eringen 1999 [7]

Since the development of non-local theories there have been attempts to identify if the size effects, noted by the theories, exist in real materials. Initial attempts to identify size effects in heterogeneous materials did not prove fruitful [9]. Indeed it is recognised as a difficult task [7], see quote above, as any experiment is trying to identify microscopic level interactions via the macroscopic response of a material under load. Gauthier and Jahsman [10] were the first researchers to separate and devise an experimental procedure to identify all six of the micropolar material constants. Analytical expressions were developed for the mechanical response

in tension, torsion and plate bending. If a micropolar material were tested at reduced sample sizes then the analytic solution predicts that, in torsion and bending, there would be relative stiffening as the sample size reduces. These size effects can be used to determine all of the micropolar material constants [10].

To test this procedure a model material was created where aluminium shot was suspended in an epoxy polymer matrix to 99.5%; it is not stated if this is by volume or weight [9, 10]. The resulting displacement in the torsion case was measured using both holographic interferometry and precision dial gauges. The torsion results proved inconclusive with a large scatter in the data and if any conclusion could be drawn it suggested that a reduction in stiffness was present, not the increase that might have been expected. This was attributed to the friction in the testing equipment and material inhomogeneity. Dynamic tests are a suggested alternative and in a later publication these tests show some presence of micropolar behaviour [10] but are unable to extract all micropolar material properties. Theoretical work conducted by Bigoni [11] may shed some light upon why Gauthier and Jahsman did not find size effects in the model material that was created. Through a homogenisation procedure Bigoni shows that, in a two phase composite, the inclusion must be less stiff than the matrix material before the material will behave in a micropolar manner. This is the opposite of the model material that Gauthier and Jahnsman manufactured. Although no size effects were found using the static test these did form the foundation for future work under the name of “the method of size effects”.

Lakes is the most prolific researcher in the field of experimental determination of micropolar material properties. In his extensive review [12] he makes note of the state of the art, as of fifteen years ago, discussing the merits and drawbacks of various approaches. The salient details mentioned are: the technique that was adopted, in which materials size effects were discovered, whether micropolar elasticity is indeed an adequate model, how the preparation of sample affects size effects and what comment his work has attracted. These will now be discussed.

Lakes advanced Gauthier and Jahsman’s work in the method of size effects by developing a magnetic torque and bending rig that could transmit the required loads without friction. Displacement was measured using a holographic inter- ferometer. Employing both a non contact loading and measurement technique

reduced the parasitic error, due to instrument friction [13]. Analytical solutions for the bending [14] and torsion of circular cylinders were used to identify the micropolar moduli. Although size effects were identified in torsion of polymeric foam, the bending of smaller samples identified a departure from micropolar elas- ticity. Lakes proposed that this could be due to additional degrees of freedom in the microstructure. Micromorphic elasticity [7], a more generalised microstruc- ture elasticity theory, may have provided a better correlation to the experimental data. In further work [15], size effects are identified in dense polyurethane foam but not in syntactic foams. It is thought that in the syntactic foam the inclusion is stiffer than the matrix. This confirms Bigoni’s hypothesis [11] as consequently the material behaves in a nearly classical manner. Micropolar moduli are also identified in compact bone [16]. Comment is passed by Eringen [7] about the measured coupling number being too high which would imply a near zero shear modulus.

Later work by Anderson and Lakes [17], analysing the size effects in closed cell polymethacrylimide, identified that surface damage during sample preparation can cause size softening rather than size stiffening. A surface damage model is incorporated into the analytic solutions for bending and torsion of circular cylinders. Surface damage effects are due to half open voids being present at the boundary of the material. The half open voids are less able to carry the load than the fully enclosed voids. As the size of the boundary increases with respect to the overall cross section of the material it is possible that an anti micropolar effect is present. Careful sample preparation can mitigate this error. There is an apparent trade off between testing a material at smaller sample sizes, where the size effect will be more pronounced and distinguishable from the systematic error of the testing procedure, and testing at such a small scale that the surface damage of the material becomes significant with respect to the overall material response.

Further to the method of size effects and dynamic tests, Lakes presented a field method for qualitatively determining the correct continuum model that the ma- terial exhibits. Analysis of the strain field on the surface of a rectangular section under torsion is presented in [18]. It was found that at the edge of the rectangu- lar section the shear stress was non zero, indicating that non classical material

behaviour is present. A screening method using a holographic image to follow the motion of a small edge crack in a rectangular beam under torsion is presented in [19]. A moving crack would be indicative of a micropolar material.

Since the review of Lakes, further work has identified size effects, in the shear modulus and damping of bovine plexiform bone [20], using Lakes torsion tech- nique. Beuchner’s work suggests that an understanding of size effects will inform upon the understanding of the scaling laws of bones, identified in larger animals, and geological structures. McFarland [21] returned to Gauthier and Jahsman’s work to retrieve the, yet unused, analytical solution for the bending of microp- olar plates to identify size effects in micro electro mechanical systems (MEMS).

A polypropylene micro cantilever beam, end loaded by a nanoindenter, showed a size stiffening up to four times greater than that predicted by classical beam theory. This work only allowed the determination of the characteristic length of bending but this is sufficient to gain a displacement field for a slender micropolar beam.

As can be seen size effects have been identified in a wide variety of materials in- cluding micro mechanical beams, biomaterials and polymeric foams, which have impact upon many fields of engineering. An adequate approach is therefore re- quired to both determine the constitutive properties of heterogeneous materials and apply them to the analysis of these materials in engineering design.

### 1.2 Numerical Methods in Micropolar Elasticity

“...bring the topic of microelastic continua from one of abstraction to that of reality...” Goldberg 1974 [22]

The finite element method (FEM), of great popularity in the field of computa- tional structural mechanics, was first turned to micropolar elasticity by Baluch,

Goldberg and Koh [23]. They formulated a bi-linear triangular element with lin- ear displacement and linear micro rotation fields. Although no numerical results are presented they note that their purpose is to bring micropolar elasticity and its associated micro continuum models from “ one of abstraction to that of real- ity”. The nature of micro continuum theories is complex and therefore very few analytical solutions exist. Goldberg [22], in a later work states that the finite element method is used “in order to alleviate the inherent complexity” involved in solving the system of governing equations. His later work presents an FEM for the bending of micropolar plates using a 3 noded triangular element with 15 degrees of freedom; transverse displacement, rotation and micro rotation.

Nakamura, Benedict and Lakes [24] present another bi-linear triangular element for orthotropic micropolar elasticity. Results are shown for the estimation of stress concentration factors of a circular hole in an infinite plate, for which an analytical solution exists. The model is capable of identifying the size effect, although there is an error in the computed value that appears to be dependent upon the coupling number; the larger the value of the coupling number, which is a constitutive property governing the antisymmetry of the shear stresses in micropolar elasticity, the greater the error. This issue is identified in other works [25, 26]. In a later work Nakamura and Lakes [27] present a finite element analysis package called MIRACS (Micro rotation and couple stress) which is used to investigate Saint- Venant end effects in micropolar elastic materials. A 3 node constant strain triangular element, a 4 node isoparametric element and an 8 node isoparametric element make up the package. Further plane elements have been published [25, 28–30]. The quadratic element of Providas and Kattis [25] is the most accurate plane finite element to date. In [25], a patch test is presented to better assess the published element. Wheel [26] departs from the standard finite element procedure to publish a constant strain planar control volume method. This method shows enhanced performance in the patch test of Providas and Kattis; returning the exact stress states for each test, which the finite element formulations were unable to.

The first three dimensional element to be developed was by Huang et al [31]; a Wilson’s non-compatibility brick element with 6 nodal degrees of freedom and 8 nodes. An interesting investigation of the role of various constitutive prop-

erties upon the computed displacement to the exact solution of a beam with a non kinematically distinct micro rotation, i.e. couple stress beam, is presented.

Large errors are reported for certain material properties used. There appears to be no discussion as to whether the author believes that this is due to numerical inaccuracy in the finite element solution or if it is not converging to the solution because the FEM is displaying behaviour that the beam solution is unable to display due to its couple stress assumptions. Their results show that as κ, a micropolar elastic constant, increases then the solution will converge to the ana- lytical, couple stress solution. In the definition of the coupling number, N , as κ tends to infinity, N tends to 1. If N = 1 the shear stresses are fully antisymmetric and thus the problem is that of couple stress theory; hence the convergence to the exact solution. Branke et. al. [32] presents a three dimensional element for micropolar elasticity, with the couple stress assumption. It is used to simulate four point bending of a textile-reinforced composite and material parameters are determined by homogenisation. Numerical homogenisation of material properties offers an alternative to physical experiments [33, 34].

Goldberg’s work was presented to motivate the use of the FEM in the engineering analysis of materials with a microstructure but identified a debate about the correct use of constitutive properties which experiments can shed light upon.

Indeed these conclusions are the same today. There is still discussion in the literature about the correct constitutive properties to use and most presented work to date has yet to find a useful application where experiments and numerical work tie up to showcase a useful analysis technique for materials with micro structure. It is the aim of this work to strive towards this goal.

### 1.3 Research Aims

Size effects have been identified previously in real materials but is micropolar elas- ticity really an adequate model to quantify this? Previous work has shown that it is difficult to distinguish size effects from experimental errors. In addition to this bespoke testing equipment is often required. To date no work has conducted the experimental determination of constitutive properties and the development of

numerical models to assist in this. Both these aspects are essential if micropolar elasticity is to be used in computational engineering analysis and design. What is discussed in this work is a designed model heterogeneous material that will be examined to see if micropolar elasticity can describe its deformation. In addition numerical techniques will be developed that will be used to assess if micropolar elasticity can be used as an appropriate analysis tool and, for the first time, used in the identification of the constitutive properties. This will be the first compar- ison between a real material, experimentally tested to determine the constitutive properties, and a numerical solution to micropolar elastic problems.

Due to the inherent complexity of heterogeneous materials and micropolar elas- ticity only one and two dimensional problems are considered. There is, however, much to be considered in these cases that will impact upon any future work moving into full three dimensional representations. Beginning with the general linear theory of micropolar elasticity, this will be reduced in complexity to look at first the bending of slender micropolar beams and secondly the bending of deep micropolar beams. Solutions to these problems, by analytical and numer- ical methods, are compared against experimental responses of a model material under three point bending at various spans using the method of size effects. In addition to the method of size effects, limited by available analytical solutions, it is proposed that advances in the computational modelling of micropolar materi- als can bring about an inverse method for identifying the constitutive properties.

This utilises a newly developed linear strain micropolar control volume element which iteratively finds the correct constitutive properties from experimental test- ing data. Further to this, the new iterative search procedure will be used to fit constitutive properties to the, experimentally determined, stiffness of diamet- rically loaded heterogeneous rings. These rings are made of a different model material.

This thesis sets out the mathematics of linear micropolar elasticity and the pro- gression to plane stress and plane strain problems, followed by the formulation for a slender micropolar beam and a thin walled micropolar ring. With the so- lution of a slender beam in place, the creation of the model material and its testing as a slender beam will be discussed. After this, a return will be made to the plane stress and plane strain formulations when a linear strain micropolar

control volume finite element will be formulated. This will then be used in the analysis of deep beams, based upon the constitutive properties gained from the slender beams, and used to identify a further constitutive property. Finally, to prove the method assembled in the analysis of thick beams, micropolar constitu- tive properties from diametrically loaded ring samples will be determined. This work therefore shows a useful application of micropolar elasticity as an analysis tool to predict the deformations of heterogeneous materials in bending.

## Chapter 2

## Micropolar Elasticity

Micropolar elasticity is one of the higher order non-local theories of Eringen [7]. It is endowed with an additional micro rotation vector that removes the restriction upon classical elasticity that the shear stresses are symmetric. It is a general model and will converge to both classical elasticity and couple stress theory. The three dimensional stress tensors of linear micropolar elasticity are introduced and the constitutive properties are discussed. Following this, and reducing the complexity, four special cases of linear micropolar elasticity are considered; the two dimensional formulations of plane stress and plane strain, the one dimensional formulation for a slender beam and the one dimensional formulation for a thin walled ring, these being the focus of the research in this thesis.

### 2.1 Generalised Linear Micropolar Elasticity

Linear micropolar elasticity takes into account the deformation of the microstruc- ture by introducing a length scale dependent couple stress, m, and an additional degree of freedom, the micro rotation φ. For a linear elastic isotropic micropolar material the force stress tensor, τij, and couple stress tensor, mij, respectively are [5],

τij = λεkkδij+ (2µ^{∗}+ κ) εij + κeijk(θk− φk) (2.1)

mij = αφk,kδij + βφi,j+ γφj,i (2.2) The repeated indices denote summation over the range (i, j, k = 1, 2, 3), δij is the Kronecker delta and eijk is the permutation tensor. These are defined in the following way:

δ_{ij} =

1, if i = j 0, if i 6= j

(2.3)

eijk=

+1, if ijk is an even permutation of (1, 2, 3)

−1, if ijk is an odd permutation of (1, 2, 3) 0, otherwise

(2.4)

An index followed by a comma represents a partial differentiation with respect to
the coordinate system. τ is the force stress tensor, m is the couple stress tensor,
θ is the macro rotation, φ is the micro rotation and λ, µ_{m}, κ, α, β, γ are six elastic
constants. µ^{∗} is the micropolar shear modulus. This is related to the observed
shear modulus µ by,

µ = µ^{∗}+κ

2 (2.5)

The macro rotation and strain tensor respectively are,

θi = 1

2eijkuk,j (2.6)

εij = 1

2(ui,j+ uj,i) (2.7)

where u is the displacement vector. The six elastic constants can be expressed in terms of seven engineering constants [12]:

Em = (2µ^{∗}+ κ) (3λ + 2µ^{∗}+ κ)

(2λ + 2µ^{∗}+ κ) (2.8)

Gm = µ^{∗}+ κ

2 (2.9)

νm = λ

(2λ + 2µ^{∗}+ κ) (2.10)

l^{2}_{t} = (β + γ)

(2µ^{∗}+ κ) (2.11)

l^{2}_{b} = γ

2 (2µ^{∗}+ κ) (2.12)

N^{2} = κ

2 (µ^{∗} + κ) (2.13)

Ψ = (β + γ)

(α + β + γ) (2.14)

where Em is the micropolar Young’s modulus, Gm the observed micropolar shear modulus, νm the micropolar Poisson’s ratio, lt the characteristic length of tor- sion, lb the characteristic length of bending, N the coupling number and Ψ the polar ratio. The micropolar equivalents of the classic elastic constants inform the behaviour in much the same way as in the classical theory. The characteristic lengths of torsion and bending dictate the length scale of the size effects. The coupling number controls the antisymmetry of the shear stresses. The polar ratio is equivalent to Poisson’s ratio but with respect to the micro rotation. The mi- cropolar theory contains two limits. If α, β, γ and κ are set to zero, the solid will behave in a classical manner. Alternatively if the coupling number N is set to 1 then the material will behave as in couple stress theory, where the micro rotation is no longer kinematically distinct from the macro rotation.

### 2.2 Two Dimensional Formulations

Reducing the complexity of the general form of linear micropolar elasticity pro- duces two dimensional formulations for plane stress and plane strain [27]. The static equilibrium equations for the balance of stress and couple stress, see figure 2.1, are respectively;

### x y

### z

### m

_{xz }

### τ

_{yx }

### τ

_{xx }

### m

_{yz }

### τ

_{yy }

### τ

_{xy }

### dx dy

Figure 2.1: Micropolar differential stress element

τij,i+ pj = 0 (2.15)

mi3,i+ eij3τij + q3 = 0 (2.16) where the repeated indices denote summation over the range (i, j = 1, 2). pj are body forces per unit volume and q3 represents a body couple per unit volume.

Expanding the equilibrium equations for Cartesian coordinates, (i, j = x, y) and setting the free index 3 to z gives;

τxx,x+ τyx,y+ px = 0 (2.17) τyy,y+ τxy,y+ py = 0 (2.18) mxz,x+ myz,y + τxy− τyx+ qz = 0 (2.19)

The linear constitutive equations can be expressed as,

### x y

### z

### ε

_{xy }

### ε

_{yx }

### φ

^{z}

### x y

### τ

_{a }

### τ

_{a }

### τ

s### τ

_{s }

### v

_{,x }

### u

_{,y }

### φ

zFigure 2.2: Deformation of stress element due to antisymmetric, τ_{a}, and sym-
metric, τ_{s}, shear stresses

τij = λεkkδij + (µ^{∗}+ κ) εij+ µ^{∗}εji (2.20)
mij = αφk,kδij + βφi,j+ γφj,i (2.21)
where the repeated indices denote summation over the range (i, j, k = 1, 2, 3).

Introducing a modified strain displacement relationship where,

εij = ui,j+ eijkφk (2.22) which expanded for Cartesian coordinates (i, j, k = x, y, z) gives,

εxx

εyy

εyx

εxy

=

u,x

v,y

u,y+ φz

v,x− φz

(2.23)

where u and v are the displacement components of the x and y directions re- spectively. The displacement gradients u,y, v,x are associated with the symmetric

component of the shear stresses, τs, while the micro rotation φz is due to the antisymmetric component of the shear stresses, τa, see figure 2.2. The constitu- tive equations are now modified to account for the specific assumptions present in both the plane stress and plane strain theory.

### 2.2.1 Plane Strain

In plane strain it is assumed that the z component of strain is zero as in the classical case. In addition for micropolar elasticity the micro rotation is assumed to be zero about the x and y directions. Therefore εzz = εxz = εyz = εzx= εzy = 0 and φx = φy = 0. This gives rise to the modified constitutive equations, expressed in expanded matrix form in the Cartesian coordinates for force stress,

τxx

τyy

τyx

τxy

=

λ + 2µ^{∗}+ κ λ 0 0

λ λ + 2µ^{∗}+ κ 0 0

0 0 µ^{∗}+ κ µ^{∗}

0 0 µ^{∗} µ^{∗}+ κ

εxx

εyy

εyx

εxy

(2.24)

and couple stress,

"

mxz

m_{yz}

#

=

"

γ 0 0 γ

# "

φz,x

φ_{z,y}

#

(2.25)
These can be reformulated in term of the engineering material constants Em, vm,
l_{b} and N from equations (2.8),(2.10),(2.12) and (2.13) respectively as,

τxx

τyy

τyx

τxy

= Em

(1 + νm)

(1−νm) (1−2νm)

νm

(1−2νm) 0 0

νm

(1−2νm)

(1−νm)

(1−2νm) 0 0

0 0 _{2(1−N}^{1} ^{2}_{)} (^{1−2N}^{2})

2(1−N^{2})

0 0 (^{1−2N}^{2})

2(1−N^{2})
1
2(1−N^{2})

εxx

εyy

εyx

εxy

(2.26)

"

mxz

myz

#

=

" _{2E}_{m}_{l}^{2}

b

(1+νm) 0
0 ^{2E}^{m}^{l}

2 b

(1+νm)

# "

φz,x

φz,y

#

(2.27) An alternative relationship between the shear stresses and the shear strains can be formulated by introducing a new constitutive parameter, the coupling factor, a, where,

N^{2} = a

1 + a (2.28)

Then expressing the shear modulus Gm as

Gm = Em

2 (1 + νm) (2.29)

allows the shear stresses to be related to the shear strains in the simpler form,

"

τyx

τxy

#

= Gm

"

1 + a 1 − a 1 − a 1 + a

# "

εyx

εxy

#

(2.30)

### 2.2.2 Plane Stress

In plane stress theory it is assumed that the stress in the z direction is zero and again it is assumed that the micro rotations about the x and y axes are zero.

Therefore τ_{zz} = τ_{xz} = τ_{yz} = τ_{zx} = τ_{zy} = 0 and φ_{x} = φ_{y} = 0. As the assumptions
with respect to the couple stress are unchanged between plane stress and plane
strain the constitutive relationships are unchanged from equations (2.25) and
(2.27). However the modified force stress constitutive relationships are,

τxx

τ_{yy}
τyx

τxy

=

(2µ^{∗}+κ)(2λ+2µ^{∗}+κ)
λ+2µ^{∗}+κ

λ(2µ^{∗}+κ)

λ+2µ^{∗}+κ 0 0

λ(2µ^{∗}+κ)
λ+2µ^{∗}+κ

(2µ^{∗}+κ)(2λ+2µ^{∗}+κ)

λ+2µ^{∗}+κ 0 0

0 0 µ^{∗}+ κ µ^{∗}

0 0 µ^{∗} µ^{∗}+ κ

εxx

ε_{yy}
εyx

εxy

(2.31)

and again expressed in terms of the engineering constants,

τxx

τyy

τ_{yx}
τxy

= Em

(1 − ν_{m}^{2})

1 νm 0 0

νm 1 0 0

0 0 _{2(1−N}^{(1−ν}^{m}^{2}^{)}_{)} ^{(1−ν}^{m}^{)}(^{1−2N}^{2})

2(1−N^{2})

0 0 ^{(1−ν}^{m}^{)}(^{1−2N}^{2})

2(1−N^{2})

(1−νm)
2(1−N^{2})

εxx

εyy

ε_{yx}
εxy

(2.32)

### 2.3 One Dimensional Formulations

In generalised linear micropolar elasticity the micro rotation is kinematically dis- tinct from the macro rotation but a simplification can be made for slender beams and rings where the micro rotation equals the macro rotation [35]. This special case is often referred to as couple stress theory in the literature.

### 2.3.1 Slender Beam

The derivation for the moment curvature relationships for a slender micropolar beam and the maximum vertical displacement under three point bending follows.

The radius of curvature, R, of a beam under pure bending, being bent through a small angle is,

1 R = dθ

dx = dφ_{z}

dx = −d^{2}v

dx^{2} (2.33)

Considering only the in plane couple stress, m_{xz} and direct stress τ_{xx}
mxz = γdφz

dx (2.34)

τxx = Ef my

R (2.35)

where Ef mis a micropolar flexural modulus. Taking the internal resisting moment equal to any externally applied moment, M , see figure 2.3,

### M M

### z

### x y

### τ

_{xx }

### m

xzFigure 2.3: Stress acting upon a one dimensional micropolar beam

M = Z

A

(yτxx+ mxz)dA (2.36)

Substituting for

mxz = γ

R (2.37)

and

τ_{xx} = Ef my

R (2.38)

,

M = 1 R

Z

A

(y^{2}Ef m+ γ)dA (2.39)

Completing the integration where the second moment of area, I is,

I = Z

A

y^{2}dA (2.40)

and area, A is

### W

### L

### d b

Figure 2.4: Model beam subjected to three point bending

A = Z

A

dA (2.41)

and substituting for

1

R = −d^{2}v

dx^{2} (2.42)

the moment curvature relationship is,

d^{2}v

dx^{2} = − M

Ef mI + γA (2.43)

From the moment curvature relationship the maximum displacement, vmax for a micropolar beam under three point bending, figure 2.4, is,

vmax = W L^{3}

48(Ef mI + γA) (2.44)

where W is the central applied load, L is the length of the beam, Ef m is the micropolar flexural modulus, I is the second moment of area, γ is a length scale dependent micropolar constant and A is the cross-sectional area. This can be

rearranged to express the stiffness, K in terms of the beam depth d, where the stiffness is the applied load W divided by the maximum displacement vmax. For a rectangular cross section, the substitutions for the second moment of area, I, and area, A, are,

I = bd^{3}

12 (2.45)

A = bd (2.46)

where b is the breadth and d is the depth. The stiffness K is,

K = 4E_{f m}b d
L

3

1 + lb

d

2!

(2.47) where lb(m) is the characteristic length in bending for a rectangular cross section,

l_{b} =

s12γ Ef m

(2.48)

For a classically elastic beam the equation for determining the maximum deflec- tion of a beam under three point bending loading is

vmax = W L^{3}

48Ef mI (2.49)

therefore the stiffness is

K = 4Ef mb d L

3

(2.50) From this, it can be seen that in equation (2.47) the expression outside the bracket is that of the classical beam equation and inside is the term associated with the micropolar stiffening. It can also be seen that as the depth of the beam increases the significance of the characteristic length reduces and the solution converges to the equation for a classically elastic beam.

### R M

o### W

### θ

### M

### x y

### z

### W

### W

Figure 2.5: Model ring subject to diametrically opposing point loads

### 2.3.2 Thin Walled Ring

The derivation for the vertical displacement in a thin walled ring with diamet- rically opposing point loads follows. The derivation will differ from that of the slender beam and begins by defining the elastic strain energy, U , in the thin micropolar ring of radius, R, as

U = 1 2

Z ^{π}_{2}

0

M^{2}

(Ef mI + γA)Rdθ (2.51)

This equation is a modification of the strain energy function derived in [35] and the other symbols have the same meaning as in the slender beam derivation.

Summing the moments about a cut made at angle θ away from the applied load W , see figure 2.5, gives the total moment as

M = W R sin θ − Mo (2.52)

From Castigliano’s theorem the vertical displacement, v, at the load point can

be gained from,

v = ∂U

∂W = 1

(Ef mI + γA)
Z ^{π}_{2}

0

M∂M

∂WRdθ (2.53)

Making substitutions for M, equation 2.52, and

∂M

∂W = R sin θ (2.54)

The vertical displacement can be expressed as

v = R^{2}

(E_{f m}I + γA)

π

4W R − Mo

(2.55)

To find the unknown resultant moment Mo, the macro rotation mo of the ring is derived, again by Castigliano’s theorem, as

m_{o} = ∂U

∂Mo

= 1

(Ef mI + γA)
Z ^{π}_{2}

0

M ∂M

∂Mo

Rdθ (2.56)

Again making the substitution for M and letting

∂M

∂Mo

= −1 (2.57)

The macro rotation is

mo = R

(Ef mI + γA)

−W R +π 2Mo

(2.58)

Assuming that there is no macro rotation, owing to symmetry where the load is applied then

Mo = 2

πW R (2.59)

Making the substitution for Mo into equation 2.55 gives the vertical displacement at the load point as

v = W R^{3}
(Ef mI + γA)

π^{2} − 8
4π

(2.60)

This equation can be rearranged to gain an expression for the stiffness K of the thin walled ring

K = πEf mb
3 (π^{2}− 8)

d R

3

1 + l_{b}
d

2!

(2.61)

where b is the breadth of the ring, d is the depth of the ring wall and lb is the characteristic length in bending as defined in equation 2.48. Similar to the slender beam formulation, the stiffness of a classically elastic thin walled ring is outside the brackets of equation 2.61 and the bracketed term governs the length scale dependent component of the stiffness.

### 2.4 Conclusion

In this chapter the constitutive, equilibrium and kinematic equations of the gen- eral linear theory of micropolar elasticity have been laid out. This was followed by the presentation of plane stress and strain micropolar elasticity which will be used in chapter 4 to derive a linear strain control volume finite element for micropolar elasticity. Further to this two, one dimensional derivations were pre- sented. The first was for determining the stiffness of slender micropolar beams, loaded in three point bending. This will be used in the next chapter to assess if a model heterogeneous material is displaying a size dependent stiffening consistent with micropolar elasticity. Further to this it will be used in chapter 5 to aid in the determination of the micropolar plane stress constitutive properties from experi- mental data gained from three point bending of heterogeneous beams of different aspect ratios. Finally using the approach set out in chapter 5 the second one di-

mensional derivation, that of a thin walled ring, will be used to obtain micropolar plane stress constitutive properties from rings of different aspect ratios.

## Chapter 3

## Model Material - Slender Beam

With the mathematical approach set out in the previous chapter for the defor- mation of a slender micropolar beam, a heterogeneous material that exhibits a size effect in bending is required. This will enable constitutive properties to be determined, using the method of size effects, and the deformation predicted by numerical procedure. In an attempt to avoid experimental difficulties associated with real heterogeneous materials an idealised model material, that is designed to mitigate errors and produce a noticeable size effect, is required.

Three factors, that will inform upon the design of the model material, have been identified in the literature. The first is the stiffness of the inclusions in the matrix material. Previous experimental work with a model material had used inclusions that were stiffer than the matrix material [10], and found no conclusive size effect.

Recent theoretical work, however, on homogenisation procedures in micropolar elasticity has identified that the inclusion needs to be less stiff than the matrix material [11], and relatively dilute within the matrix. Therefore a material with compliant inclusions is sought. The second is the size of the inclusions with respect to the overall test sample size. If the inclusions are too small then any micropolar material response will be masked by systemic errors inherent in the test procedure [12]. If the inclusions, however, are too large, in comparison to the overall sample size, then local loading effects may become significant. The material would be better modelled as a classical continuum with all the discrete

### P

_{2 }

### P

1Figure 3.1: Diagram of hole pitch with horizontal pitch P_{1} and vertical pitch P_{2}

detail present, as a micropolar continuum assumption would break down. The third issue is sample preparation [17], mitigating any potential anti size effect.

This can be achieved by having minimal surface damage around the boundary of the test sample, ideally with no broken voids on the boundary.

In addition to these desirable material attributes a suitable testing procedure is also required. As stated above, systematic errors in the testing procedure can mask any size effect. In previous work low friction force application and non contact measurement techniques have been employed to mitigate this. It was, however, a desire of this work to use standard materials testing equipment to allow easy reproduction of these tests in the future.

The model material was chosen to be an aluminium matrix with circular voids.

The aluminium was alloy 6082 T6 with an elastic modulus of 70GPa. Standard aluminium bar stock of sizes 12.7, 25.4, 38.1 and 50.8 mm depth and a common breadth of 12.7 mm was used. Holes were drilled through the breadth in a regu- lar hexagonal pattern. The void pattern is designed in such a way that no voids intersect the boundary of the top and bottom edges of the bar. Two pitch sizes were made to experimentally determine how this might influence the size effect

Figure 3.2: Photograph of HMD test pieces

in bending. A lower mass density (LMD) and higher mass density (HMD) set of sample were made by maintaining the same void radius and vertical packing while the horizontal pitch was altered. Figure 3.1 shows the void pitch measure- ments and table 3.1 gives dimensions for the sizes of the void pitches. This model material is anisotropic due to the hexagonal packing and different horizontal and vertical pitches. The length of the test samples where such that they could be tested at an aspect ratio of approximately 10:1, (length:depth). This allows a slender beam assumption to be made, meaning that the dominant mode of defor- mations is due to bending and any shear deformation is minimised. A size effect in bending can be identified by varying the depth of a beam while maintaining the same aspect ratio of length relative to depth. If the beams were behaving in a classical manner then the stiffness of the sample should remain constant. For a micropolar material, however, the stiffness should increase with a reduction in depth. This is demonstrated mathematically in section 2.3.1. To this end test pieces of four different depths were manufactured for each density, dimensions of which can be seen in table 3.2. The four HMD test pieces can be seen in figure 3.2.